using self-assembled monolayers that present .using self-assembled monolayers that present...
Post on 05-Sep-2018
Embed Size (px)
using Self-Assembled Monolayers That presentOligo(ethylene glycol) Groups To Controlthe Interactions of Proteins with Surfaces
Milan Mrksich'and George M. Whitesides'
'Department of Chemistry, University of Chicago, 5735 South Ellis Avenue,
Chicago, IL 60637'Department
of chemistry, Harvard university, l2 oxford street,Cambridge, MA 02138
This chapter rev iews the use of se l f -assembled monolayers o falkanethiolates on gold to control the interactions of proteins and cel lswi th man-made mater ia ls . The work is based on the ab i l i ty o fmonolayers that present ol igo(ethylene glycol) groups to resisi thenon-specific adsorption of protein. The chapter desciibes the use offunctionalized monolayers for the bio- and chemo-specific adsorptionof proteins. The chapter concludes with a discussion of techniquesthat can p-attern the formation of monolayers and that can preparetailored substrates for the control of cell attachment.
The property of.poly(ethylene glycol) (PEG) to resist the non-specific adsorption ofprotein has made this material the standard choice for applicaiions requiring inertsurfaces. There el lst a variety of excel lent strategies for^tai lor ing the^surfa"ces ofmaterials with PEG. Most of the methods of using PEG are emprrical. and amechanis t ic unders tanding of the ab i l i ty o f PEG io res is t adso ip t ion is s t i l lincomplete. As a consequence, the structural parameters of PEG that make surfacespresenting i t unable to adsorb proteins (that is. inert to adsomtion) are st i l l not wellunderstood, and i t is not yet routine to design new inert materials-or even simplederivatives of PEG-frornbasic principles.
We have used self-assembled monolayers (SAMs) of alkanethiolates on gold thatpresent oligomers of the ethylene glycol group (-EGnoH, n = 2-6, and -EG6dCH3) asmodel surfaces with which to study the properties of materials tailored with PEG 11-4). Several considerations make this class of SAMs the best that is currently availablefor fundamental studies of the relationships between the structure of a material and itsinterfacial properties. The structure of these interfaces is reasonably well-defined andstable over the intervals required for experiments involving protein adsorption andcell attachment. They.can-be systematic-ally tailored using ioutine organic'syntheticmethods (4-6). Addit ional considerations that make this system pait iculariy well-suited for studies of bio-interfacial phenomena include the-use of surface piasmonresonance spectroscopy to measure the association of proteins with monolayers (3)and of microcontact printing to pattern the formation of monolayers ( D.
This -chapter rev iews our work that has used monolayers present ingoligo^(ethylene glycol) groups to control the interaction of proteins and^ cells wit[interfaces. The chapter begins with an introduction to SAMs, then discusses the
O 1997 American Chemical Society 361
362 POLY( ETHY t ,E \E GL \ ' ( 'O I , )
properries of SAMs presenting ol igo(ethylene gly.col) groups, the interactions of
oroieins q' i th functional ized SRHns, and methodologies that use techniques from
microfabrication to create substrates that control the attachment of cells'
Alkanethiolates on Gold. Self-assembledgold form upon the adsorption of long chainn = 11-181 flom solution (or vapor) to a gold
Self-Assembled MonolaYers ofmonolayers of alkanethiolates onalkanethiols, RSH [R = X(CH2)n,surface:
RSH + Au(O)n---> RS-Au(I)'Au(0)n + 1/2H2Q) (eq 1)
Extensive experimental work has shown that the sulfur atoms coordinate to the three-fold sites of the gold(111) surface and the close-packed alkyl ch1.ns are trans-extended and tilted-approximately 30" from the normal to the surface (Figure 1)' Theterminal functional grbup X is piesented at the surface and determines the propertiesof the interface. Th"e prbperties of SAMs can be controlled further by formation of"mixed" SAMs from solutions of two or more alkanethiols.
Kinetics of Formation of Monolayers. The mechanisms for the assembly ofmonolayers are complex and not completely understood. _several gr.oups h.ave studiedthe kinetics for assembly of alkanethiolaies on gold (8-11). This work has useddifferent methods, and alihough the data are not entirely consistent, most indicate thatgreater than gOVo of the monolayer forms quickly-within minutes for mM solutions5t tttiot-and the remainder forms more slowly over hours. The kinetics for theinitial, rapid assembly of the monolayer are probably domrnated by the interactionbetween the thiolate and gold substrate and gives a monolayer that is locally orderedbut contains defects. We presume that the second, slower phasg of assembly invoh'esthe reordering of alkanethiolates on the surface and transfer of alkanethiol moleculesfrom solutionto the remaining vacant sites on the gold substrate.
For many terminal groupi, the differences in properties of the monolavers formedunder differ6nt conditlons'are minor; the contact angle of water on SAMs ofoctadecanethiolate, for example, is insensitive to the differences in structure of thephases formed in the terminal stages of assembty (2). For SAMs presenting othergtoupr, however, the properties can change dramatically with increasing dens.ity ofittuti"itriolates. tn a subsequent section we describe differences in the adsorption ofprotein to SAMs presenting oligo(ethylene glycol) groups that depend on thepreparation of the monolayers.
Theory of the Mechanisms Underlying the Ability of PEG to Resist Adsorptionof Protein. In aqueous solution, poly(ethylene glycol) chains _are solvated anddisordered; measurements using NMR spectroscopy (12) and differential thermalanalysis (/-l) indicate that as many as three water molecules are associated with eacht.p"ht unlt.
'Fu.ther evidence forihe large_excluded volume of PEG comes from gel
chromatography experiments that show PEGs are substantially larger than otherpolymers-of si.nita.^molecular weight (14). De Gennes and Andrade have_proposedihai surfaces modified with long PEG chains resist the adsorption of protein by "stericstabilization" (.15,16). Adsorption of protein to the surface causes the gly-col chains tocompress, with concomitant desolvati,on. The energetic penalty of transferring waterto th^e bulk and the entropic penalty incurred upon compression of the layer both serveto resist protein adsorPtion.
Analytical Methods that Measure Adsorption. Experimental studies of proteinadsoiption require analytical methods that can measure adsorption with highsensifivity; for exampl-e, I\Vo of a monolayer of a globular protein having amoleculai weight of 30 kD corresponds to a density 9f
-0.3 ng/mm2. It is alsopreferable that the techniques measure adsorption in real time to provide kinetic data
23. MRKsrcH & wHTTESTDES SAMs That Present Oligo(ethylene glycol) 363
and are non-invasive in that they do not affect or damage the layer of adsorbedprotein. Several group_s_have used techniques based on ellipsomeiry e,2), quartzcrystal microbalance (17), surface acousti-c waves (17), waieguide inieifeioinetry(19), and surface plasmon resonance (SPR) (J). Ellipsometry r"emains a convenienttechnique for measuring the amount of protein on substrates ihat had been removedfrom solution and dried; it is less convenientfor in sirz measurements. SpR fulfillsall of these criteria and has the additional advantage that instruments are nowavailable from commercial vendors. Because SPR itsJlf uses thin films of gold, it iswell-suited for characterizing adsorption on monolayers of alkanethiolates.
SAMs PresentinS. plig_o_lgthylene glycol) Groups Resist the Non-specificAdsorption of Protein. We have used honolayers fhat present short oligorirers ofthe ethylene. glycol gro.uq to inve-stigate the basis for PEG'to resist the ads6rption ofprotein (1-3)' Our work has used m1x.ed S_AlvIs plgparea from solurions contiining afunctionalized alkangt!1ol (HS(cq?)11(o_cH2cHi;noH, n=2-6) and a methll-terminated alkanethiol (HS(CHz)roCH:). This-system permits control over both rhelengthand density.of glycol chains at the-surface-(Figur'e 2). Because adsorption candepend dramatically on the structure of a proteinllg), we have used a^panel ofrepresentative proteins to characlerrze these monolayers. Both ex sira ellipsometryand in situ SPR show.that SAMs^presenting_only oligo(ethylene glycol) g.oup, resiitalmost entirely the adsorption^ofprotein.
-Extensivi *ork in olilaboritory shows
that these surfaces are very effective in resisting adsorption of proteins, and evenresist adsorption from concentrated (1-10 mg/ml-) solutions of mixtures of protein.Mixed. SAMs presenting this group togeth; wiih as much as 50Vo hydrophobic,methyl groups also resist.the adsorption.-o.f protein; SAMs presenting methyl'groupsalone adsorb most proteins.rapidly and irieversibly. The^ability o? ttr" surf-ace ioresist adsorption increases with-both the density and iength of the ,i6go-...
Mechanisms of Inert SAMs. Our work shows that surfaces presenting denselypacked short oligomers.of the.ethylene glycol group are highly eif.ctiue airesistingthe_adsorption of protein. It is not clear ihat iire mechanijmi for this resistance ofSAMs presentingshort,.oligo(ethy.lene glycol) chains are similar to those for highmolecular ryeiglt PEG. The exteniive solvation of PEG by water molecules is almostcertainly critical to the properties of the bulk polymer, but SAMs presenting densepacked oligo(ethylene glycol) groups probabiy io not have suffi. i .nt volume roaccommodate extensive solvation. Molecular modeling studies even suggest that theperfectly ordered SAMs cannot include any solvent eb). Because tfre l iycot chainsin the monolayers are each covalently tethered to the surface. these